established for a thickness that roughly corresponds to half the distance between the two electrodes. Further quantitative analysis of the data with a differential method leads to the conclusion that charge-transport properties at room temperature are affected by a discrete trap level pointing at 0.48⫾0.02 eV above the valence band.

DOI:10.1103/PhysRevB.77.115205 PACS number共s兲: 71.20.Rv, 72.80.Le, 72.20.Jv

**I. INTRODUCTION**

Rubrene, a tetraphenyl derivative of tetracene, has shown
to form high quality single crystals that present high
mobility^{1,2}due to a very low density of defects and impurity
related traps^{2} and to cofacial*-stacking interaction in the b*
direction resulting in a very efficient electronic coupling.^{3}
This kind of organic solid is useful not only for device ap-
plications, but also for exploring the intrinsic properties of
organic materials and investigating the upper limit of mobil-
ity in organic systems, since their characteristics are not af-
fected by the imperfections of the film structure. The electri-
cal properties of rubrene single crystals under field-effect
conditions are now well documented.^{4–7} However, even if
the transistor structure provides a useful tool to analyze the
charge transport in the regime of high charge density,^{8} it
cannot be used to determine the bulk parameters of the crys-
tals, for which other techniques have to be employed. One of
these is the analysis of the current-voltage*共I-V兲 curves by*
means of the space-charge-limited current共SCLC兲 model,^{9,10}
an easy-to-handle method that, when properly managed, al-
lows the determination of several charge-transport param-
eters, including mobility, density of free carriers, and con-
centration and energy distribution of traps. However, a strict
way of conduct must be followed in order to avoid misinter-
pretation of the data.

In this work we present an electrical characterization of rubrene single crystals grown by physical vapor transport in a flowing stream of argon. Low thermal load deposition of gold on one surface of the crystals provided good Ohmic contacts with negligible nonlinear contribution. A set of elec- trical bulk parameters for the preferential growth direction is extracted from the experimental curves with a SCLC analy- sis. Particular attention is dedicated to the trap-free regime of these curves, from which it is possible to estimate the free- electron drift mobility and the density of the traps. We also show that the response of the crystals can be interpreted in

terms of a discrete trap level at 0.48 eV above valence band
edge, in good agreement with that recently found by means
of temperature-dependent space-charge-limited current
spectroscopy.^{11}

**II. EXPERIMENTAL TECHNIQUES**

The rubrene crystals were grown by physical vapor
transport^{12}under a stream of argon and using proper cleaning
process for all the glasses to avoid contamination with or-
ganic substances. This technique offers high quality crystals
with large flat surfaces that are suitable for field-effect tran-
sistor fabrication. The crystal structure has been reported in
the literature.^{13,14}Rubrene crystals employed for the present
study have tabular morphology with a well-developed共100兲
face with well-defined width, and elongated parallel to the
关010兴 direction 关see Fig.1共a兲兴. Under the growth conditions
described above, rubrene crystallizes in an orthorhombic
*phase with unit cell parameters a = 26.86 Å, b = 7.19 Å, and*
*c = 14.43 Å, containing four molecules arranged in a herring-*
bone motif in the共100兲 plane and forming layers along the
*a-axis direction with spacing a/2=13.43 Å.*^{13}Because these
crystals present higher mobility in the direction along the
共100兲 face, we have used a gap-type geometry with two pla-
nar gold electrodes共approximate thickness of 30 nm兲 made
by vacuum evaporation from an electrically heated tungsten
wire. The gap was defined by a 25m diameter gold wire
shadowing the semiconductor surface. To reduce the thermal
load on the crystal surface during the deposition process, we
used a thin tungsten wire *共=0.5 mm兲 and small metal*
plates to mask the infrared radiation emanating from the
warmest part of the wire. All the measurements were per-
*formed in the bc plane of the crystals, in dark and under*
argon atmosphere with a Keithley 4200 semiconductor pa-
rameter analyzer, using a linear stepwise increase of the

applied voltage and measuring the quasiequilibrium current
共the transit time of the electron is less than the period of the
applied electrical signal兲. The maximum applied voltage was
210 V corresponding to an electric field of 8.4⫻10^{4}V/cm.

After each measurement the sample was left in argon atmo- sphere for a few minutes to avoid heating by Joule effect.

The surface morphology of the crystals and the parameters of
the channels共shape and real length兲 were investigated using
*a Digital Nanoscope IIIa atomic force microscope*共AFM兲 in
tapping mode, whereas the crystal dimensions were deter-
mined with the aid of an optical microscope Olympus
SZX12 coupled to an imaging software共except for the sub-
micron samples, the thickness of which were determined
with the AFM兲. Figure1 shows the optical and morphologi-
cal analyses of a representative crystal. The AFM analysis
关Figs. 1共c兲–1共e兲兴 shows the shape of the channel and the
morphology of the crystal surface关the thickness of the steps
in Fig.1共d兲 *corresponds to the value a*/2兴, while the optical
microscope image关Fig.1共a兲兴 points out the homogeneity of
*the channel and its lateral dimension W.*

**III. RESULTS AND DISCUSSION**
**A. Charge injection**

Prior to SCLC analysis, we checked the quality of the
gold contacts. Good contacts should behave as infinite reser-
voirs of charge, so that only a negligible fraction of the ap-
plied voltage is absorbed across the interface. When this con-
dition is fulfilled, the total current across the crystal is
dominated by the bulk properties of the sample.^{15}Two rep-
resentative examples are illustrated in Figs. 2 and 3 for a
good and a bad contact, respectively. Since the area and the
quality of both contacts will unavoidably present some dif-
*ferences, the unsymmetrical character of the I-V curve in*
Fig.3can be interpreted as the sign that the current is limited
by the contacts. Conversely, the perfectly symmetrical curve
in Fig.2tells us that the current in this case is limited by the
bulk of the crystal; that is, the current is bulk limited rather
than contact limited. The linear共Ohmic兲 regime at very low
bias 共inset in Fig. 2兲 also indicates that the nonlinear
Schottky barrier formed at the metal-semiconductor interface
is in this case negligible. This behavior shows that a low
FIG. 1.共a兲 Optical microscope
共a兲 and AFM 关共b兲 and 共c兲兴 images
of a rubrene crystal equipped with
two gold planar contacts defined
by means of a 25m shadow
mask. 共b兲 is a general and 共c兲 a
close view of the channel共d兲 and
共e兲 are the respective profiles.

thermal load evaporation of gold on the surface of the crys- tals can provide good contacts. In all the remainder of the work, such crystals, for which unsymmetrical curves were recorded, were systematically disregarded.

**B. Space-charge-limited current in a gap-type structure**
Two basic architectures can be used for a SCLC analysis:

the sandwich-type geometry 关three dimensional 共3D兲兴, in
which the electrodes are on the opposite face of the semicon-
ductor, and the gap structure关two dimensional 共2D兲兴 where
both electrodes are deposited on the same side of the film共or
crystal*兲. As pointed out by Grinberg et al.,*^{16} two limiting
cases can be considered in the gap structure. In the first one,
*the thickness h of the semiconductor is very small**共h→0兲,*

*where L is the distance between the two electrodes, W the*
*width of the channel, and h the thickness of the sample.*^{is}
the mobility, * the permittivity, and V the applied voltage.*

The general feature of the current flow in a thin film is,
therefore, an Ohmic behavior at low applied voltage fol-
*lowed by a transition to a new regime in which I**⬀V*^{2}*/L*^{2}, in
contrast to the 1*/L*^{3}dependence expected from the 3D analy-
sis. Following Geurst,^{17}it is possible to explain this behavior
by looking at the electric field perpendicular to the semicon-
ducting layer and therefore perpendicular to that one driving
*the charges over the distance L.*

On account of the previous considerations, it is plausible
*to assume that a single crystal of thickness h**0 with both*
electrodes on the same face is in an intermediate situation
between the 2D and 3D cases, depending on the ratio be-
*tween the two parameters h and L; when varying the ratio*
*h**/L, the coefficient in the Mott–Gurney’s equation actually*
assumes a different weight with respect to 2/. Accordingly,
it can be expected that the 2D law will dominate as long as
*h**/L1, while the 3D law will be valid when h/L1, or*
more precisely as long as*共9/8兲共h/L兲共2/*兲.

A common practice to discriminate between the two lim-
iting cases consists of plotting the current at a given voltage
as a function of the electrode distance, which is expected to
*vary as L*^{−2} in a film structure*共hL兲 and as L*^{−3} in a bulk
structure*共hL兲.*^{13}Unfortunately, such an analysis could not
be performed with our data. The reason is that the transition
*point between the Ohmic and SCLC regimes increases as L*^{2}
共see below兲. With the technique used in this work, where the
length of the channel is defined by a mask made of a cali-
*brated gold wire, practical values of L were 25*^{m, 50}^{m,}
and above. The transition can therefore be expected to be
four times larger with 50m than with 25m, with the
consequence that the SCLC regime starts outside the ex-
plored voltage共0–200 V兲; so we had to restrict our analysis
*to devices with L = 25*^{m.}

To bring evidence for a transition between the film and
bulk regimes we have analyzed the dependence of the free-
electron mobility *共the mobility extracted from the I-V*
curves in the trap-free regime, that is, after the sharp current
increase due to trap filling兲 on the crystal thickness using
both Eqs.共1兲 and 共2兲. Figure4illustrates the variation of the
calculated mobility for crystals with various thicknesses and
identical channel lengths*共L=25*m兲. It can be seen that, for
FIG. 2. Current vs applied voltage for an Ohmic rubrene-gold

system. The inset shows the lack of non-Ohmic effect of a low voltage.

FIG. 3. Current vs applied voltage for an asymmetrical rubrene- gold contact with the inset showing problem linked to the different behavior of the contacts.

thicknesses comparable to or greater than the channel length
共15m⬍h⬍40m兲, the Mott–Gurney law gives a thick-
ness independent mobility of around 3.5 cm^{2}/V s. At lower
thicknesses, a sharp rise of the calculated mobility occurs.

This is because, when the cathode-anode spacing becomes
larger than the crystal thickness, Eq. 共2兲 loses its physical
meaning and, although it is an approximate description of the
system, the Geurst law has to be used共a more reliable theory
would have to consider the finite thickness of the crystal兲. A
converse behavior is followed by the 2D mobility; that is, at
low thicknesses, the 2D mobility magnitude is comparable to
that of the 3D mobility at high thickness, while it tends to
depart from this mean value as the thickness increases. In
conclusion, Fig.4brings evidence for a transition between a
2D and a 3D regime. The fact that the transition point occurs
*at h⯝13*m, that is, when *共9/8兲共h/L兲⯝共2/*兲 brings addi-
tional evidence for such a transition.

We note that above the transition point, the 3D mobility is independent of the thickness of the crystal, which can be interpreted by stating that the current density is uniform over the whole section of the crystals. At this point, the question arises as to how can the charge carriers be uniformly injected in the whole thickness while the contacts are only located on one side? 3D modeling would be required to give a definitive answer to that, but we can put forward a simple image where the mobility in the direction across the crystal of the charges is high enough to provide a uniform repartition of the in- jected charge. Of course, such a process would not operate for very thick crystals; however, this limitation is not reached in the present case.

**C. Bulk parameter extraction**

Within the thickness domain where the Mott–Gurney model provides a good description of the system, a set of electrical parameters is easily extracted from the experimen- tal curves. We show in Fig.5a representative experimental

*I-V curve in linear and double-logarithmic scales.*

At low voltages, the curve follows an Ohmic共linear兲 re- gime, due to the presence of thermal free carriers related to shallow defect states, that at room temperature does not act like effective charge traps. Upon increasing the applied volt- age, a transition from this regime to a square law regime occurs. From the Mott–Gurney theory we know that such a trend can be described by

*J =*9
8⑀^{V}^{2}

*L*^{3}, 共3兲

where the trap parameter *= n/共n+n**t*兲 is the ratio between
*the density of free carriers achieved under injection, n, and*
*the total density of injected carriers, trapped n** _{t}*, and free.

Therefore this regime is linked to the presence of a discrete
trap level that reduces the measured 共or effective兲 charge
carrier mobility *ef f*= and affects the space-charge-
*limited current. Note that if n*_{t}*n, the trap parameter re-*
duces to*⯝n/n**t**. Given the voltage V*_{⍀}_{⬘} at which the tran-
sition between the Ohmic and SCLC regimes with traps
occurs, an estimation of the thermally generated electron
density *n*_{0} is possible by using the equation *n*_{0}

*= V*_{⍀}_{⬘}*V/eL*^{2}. At higher voltages, the current experiences an
almost vertical rise 共as predicted by the Lambert regional
approximation method兲 and reaches the so-called trap-free
*regime at an applied voltage V**TFL**= eN**t**L*^{2}*/, where N**t*is the
*density of traps and e the elemental charge. Actually, at V**TFL*

the amount of charge injected by the contact is sufficient to fill the traps, so that the quasi-Fermi level establishes at a level above the trap distribution within the energy gap; ac- cordingly, the mobility is no more affected by impurity or FIG. 4. Calculated mobility vs crystal thickness as derived from

Eqs. 共1兲 and 共2兲. The channel length is constant and equal to
25m. The mobility value extracted with the Mott–Gurney law for
the thick samples is approximately equal to 3.5 cm^{2}/V s.

FIG. 5. Current density vs applied voltage in double-logarithmic
and linear共inset in the figure兲 scales for an ⬃13m thick rubrene
single crystal at room temperature. Four different regimes are
clearly observable:共i兲 at low voltage the current rises linearly and
共ii兲 becomes SCL at higher field. Up till the 共iii兲 transition point
*V** _{TFL}*the properties are still determined by traps, to the point they
become filled and a regime given by the Mott–Gurney law共iv兲 关see
Eq.共2兲兴 takes place.

defects states. Under such circumstances, all additional car-
riers introduced are essentially free, so the free-electron mo-
bility can be estimated from Eq.共3兲 with= 1. Access to
the trap-free mobility is obtained in the rare case when the
density of trap is significantly low 共otherwise the semicon-
ductor is damaged before that limit is attained兲. We note also
*that the knowledge of V** _{TFL}*makes it possible to estimate the

*density of traps N*

*t*

*from the experimental I-V curves. How-*ever, it should be pointed out that this is only valid under the assumption that the traps are uniformly distributed in the volume of the crystal, which is most often an oversimplifi- cation, because the density of traps at the interface is always different from that in the bulk.

^{8}

When analyzing the experimentally determined triangle of
Lampert and Mark^{9} reported in Fig. 5, we also see that the
presence of shallow trapping delays the finish of the Ohmic
*regime from the critical voltage V*_{⍀} *to V*_{⍀}_{⬘}=共1/*兲V*_{⍀} in
agreement with the discrete trap level theory 共the ratio be-
*tween V*_{⍀}*and V*_{⍀}_{⬘}is equivalent to兲.

All the curves used to estimate the reliance of the mobility
on the crystal thickness 共Fig. 4兲 present the same trend: a
square-law dependence at low voltage followed by a sharp
current increase and a second square-law region at higher
*current. The I-V curve for a 560 nm thick rubrene crystal is*
reported as a further example in logarithmic and linear scales
共Fig. 6兲. The trap-free region is preceded by a square-law
section and by an increase of the current due to trap filling.

We also observe a second vertical rise, a characteristic found also in some thick crystals, that could represent either the filling of another discrete trap level, or the breakdown of the system at high injected current density.

The electrical parameters for two thick crystals are given
in TableI. All the numbers are extracted by analyzing the
*experimental I-V curves with Mott–Gurney’s equation*关Eq.

共3兲兴. The trap constantis calculated from the ratio between
the effective *ef f* and trap-free mobility, but the same
*value can be found by considering that in the log J − log V*
plot the trap limited curve is shifted below the trap-free curve
by*. The density of thermal carriers n*_{0}is estimated knowing

*and the transition potential V*_{⍀}_{⬘}. The in-plane rubrene static
dielectric constant was assumed to be *r*= 2.6, the mean
value extrapolated from the crystal full dielectric tensor at

^{= 0.}^{20}

**D. Space-charge-limited current differential method:**

**The discrete trap level energy**

To avoid incorrect interpretation of the SCL trend in the
*I-V curves, but also because in many samples the complete*
trap-free regime is followed by an electrical breakdown共Fig.

7兲, we have also analyzed the characteristics in terms of the
SCLC differential method.^{21} This technique, a general start-
ing point for determining bulk localized states,^{22}is based on
the assumption that on changing the position of the quasi-
*Fermi level E**F* 共by increasing the voltage applied to the
sample兲, one can determine the distribution of traps for
which the occupancy is changed. Moreover it represents a
straightforward tool to prove the consistency of the experi-
*FIG. 6. I-V characteristic of a 560 nm thick rubrene crystal with*

gold electrodes on the surface and a channel length of 25m in double-logarithmic scale and linear scale共inset in the figure兲. The inset shows the complete experimental characteristic, whereas, for clarity, in the logarithmic plot only the SCLC behavior is reported.

FIG. 7. Current vs applied potential in a rubrene single crystal.

The trap-free regime is followed by a breakdown of the system.

This event could lead up to misunderstanding and bad interpretation of the vertical rise that precedes it.

mental results with the simple Mott–Gurney discrete trap
SCLC model and to exclude any misinterpretation of the
data, such as assigning the square-law dependence to a dis-
crete trap level instead of a monotonously increasing slope,^{10}
followed by double injection effects.^{9,23,24}

In the framework of the SCLC analysis, using the zero-
temperature statistic, it is possible to estimate the parameters
of an arbitrary distribution of traps, knowing the function
*describing the distribution h共E**F*兲

*h共E**F*兲 = 12⑀^{V}

*2eL*^{2}*kT共m − 1兲* 共4兲

and the position of the quasi-Fermi level at the noninjecting
*electrode E**F**共L兲 as follows:*

*E**F**共L兲 = kT ln* *L*

1*N*_{v}*e*^{+ kT ln}*J*

*V*. 共5兲

*Here, m = d ln J/d ln V, L is the distance between the elec-*
*trodes, N** _{v}*the effective density of states in the highest occu-
pied molecular orbital, and the parameters1and2are the
average distance of the injected charge from the anode and
the ratio of the carrier concentration at the anode to the in-
jection carrier concentration, respectively. These parameters
are related to the slope of the characteristic by the
equations

^{25}

1=*2m − 1*

*m* , 共6兲

2= *m − 1*

*m* *共1 + B兲,* 共7兲

*where B is a second-order correction that can be neglected to*
a first approximation.

Equations共4兲 and 共5兲 allow us to extract, in principle, an
energy distribution of states directly from a single experi-
*mental I-V curve. However, an obvious problem is that, ac-*
cording to Eq.共5兲, the effective density of states N*v* should
be previously known in order to find the correct values of the
trap energy depth. This need, combined with the approxima-
tion of uniformity in the trap distribution, makes the calcu-
*lated trap depth E**t* only an estimation of the real value, al-
*tered by an error that may be as great as several kT.*

However, the found distribution, if correctly fitted, can be used to properly assign the SCL behavior and hence confirm the reliability of the parameters obtained with the Mott–

Gurney analysis.

*With this in mind, taking N** _{v}*= 1⫻10

^{21}cm

^{−3},

^{26}we have used Eqs.共4兲 and 共5兲 to estimate the density of those traps whose occupancy changes during the voltage sweep. For that, we have performed a fitting of the data with the bell- shaped distribution derived by Nešpurek to explain the effect

of the temperature on the visibility of discrete trap levels as follows:

*n**t**共E**F**兲 = N**t*

exp冉^{E}^{t}*kT*^{− E}* ^{F}*冊

冋^{1 + exp}^{冉}^{E}^{t}^{kT}^{− E}^{F}^{冊}册^{2}^{,} ^{共8兲}

*where n*_{t}*共E**F**兲 is the density of trapped carriers, N**t**and E** _{t}*are

*the density and the energy depth of the discrete trap, and E*

*the quasi-Fermi level given by Eq.共5兲. N*

_{F}*t*

*and E*

*t*are in this case the fitting parameters. Actually, fitting the data with this equation is possible because the experimentally accessible

*parameter is not the energetic distribution h*

*共E兲, but the den-*

*sity of trapped carriers n*

_{t}*共E兲 关strictly speaking, Eq. 共*4兲 is only valid at low temperature, under the zero-temperature

*approximation where h共E兲⯝n*

*t*

*共E兲兴. Figure*8 shows the en- ergetic distributions 共scattered data兲 and the fitting curves 共dashed lines兲 for two different samples. It can be seen that the distributions are satisfactorily fitted to Eq. 共8兲 at room temperature

*共T=300 K兲. This confirms that within the volt-*age explored, the SCL features are essentially related to a

*discrete trap level located at E*

*t*= 0.48⫾0.02 eV above the

*valence band and with a density N*

*t*=共4⫾2兲⫻10

^{14}cm

^{−3}共the uncertainty is estimated from the spreading of the fitting pa- rameters from one crystal to the other兲. A comparable dis- crete trap state level at about the same energy was found in the density of states共DOS兲 of rubrene recently reported by

*Krellner et al.*

^{11}

It is worth remembering that the thus derived trap distri-
bution is only valid in the region of the forbidden energy gap
FIG. 8. Density of states关Eqs. 共4兲 and 共5兲兴 and fitting curve to
Eq.共8兲 for two different crystals. The band edge is chosen as the
*reference level. Using the room temperature value kT = 25*

⫻10^{−3}*eV, the following fitting trap parameters are obtained: N*_{t}

= 4⫻10^{14}cm^{−3}*and E** _{t}*= 0.485 eV

*共data on the left hand side兲, N*

*t*

= 5.1⫻10^{14}cm^{−3} *and E** _{t}*= 0.462 eV 共data on the right hand side兲.

We have removed from the DOS reconstruction the apparent distri-
bution maxima appearing in the low-energy region when it falls
down the necessary condition*1.*

may be guessed that, if higher-energy states could be reached, that is, higher voltages could be applied, even greater mobility values would be found.

*the I-V curves, we have also found that the room temperature*
electrical features are related to a discrete trap level at
0.48⫾0.02 eV above the valence band.

*Also at Università di Milano-Bicocca, Dipartimento di Scienza dei Materiali, Milano, Italy; daniele.braga@mater.unimib.it

†horowitz@univ-paris-diderot.fr

1V. Podzorov, E. Menard, A. Borissov, V. Kiryukhin, J. A. Rogers,
**and M. E. Gershenson, Phys. Rev. Lett. 93, 086602**共2004兲.

2R. Zeis, C. Besnard, T. Siegrist, C. Schlockermann, X. L. Chi,
**and C. Kloc, Chem. Mater. 18, 244**共2006兲.

3D. A. da Silva Filho, E.-G. Kim, and J.-L. Bredas, Adv. Mater.

**共Weinheim, Ger.兲 17, 1072 共2005兲.**

4A. L. Briseno, S. C. B. Mannsfeld, M. M. Ling, S. H. Liu, R. J.

Tseng, C. Reese, M. E. Roberts, Y. Yang, F. Wudl, and Z. N.

Bao, Nature**共London兲 444, 913 共2006兲.**

5C. Goldmann, C. Krellner, K. P. Pernstich, S. Haas, D. J. Gun-
**dlach, and B. Batlogg, J. Appl. Phys. 99, 034507**共2006兲.

6A. L. Briseno, R. J. Tseng, M. M. Ling, E. H. L. Talcao, Y. Yang,
F. Wudl, and Z. N. Bao, Adv. Mater.**共Weinheim, Ger.兲 18, 2320**
共2006兲.

7T. Takenobu, T. Takahashi, J. Takeya, and Y. Iwasa, Appl. Phys.

**Lett. 90, 013507**共2007兲.

8R. W. I. de Boer, M. E. Gershenson, A. F. Morpurgo, and V.

**Podzorov, Phys. Status Solidi A 201, 1302**共2004兲.

9*M. A. Lampert and P. Mark, Current Injection in Solids*共Aca-
demic, New York, 1970兲.

10*E. A. Silinsh, Organic Molecular Crystals: Their Electronic*
*States*共Springer-Verlag, Berlin, 1980兲.

11C. Krellner, S. Haas, C. Goldmann, K. P. Pernstich, D. J. Gun-
**dlach, and B. Batlogg, Phys. Rev. B 75, 245115**共2007兲.

12R. A. Laudise, C. Kloc, P. G. Simpkins, and T. Siegrist, J. Cryst.

**Growth 187, 449**共1998兲.

13O. D. Jurchescu, A. Meetsma, and T. T. M. Palstra, Acta Crystal-
**logr., Sect. B: Struct. Sci. 62, 330**共2006兲.

14B. D. Chapman, A. Checco, R. Pindak, T. Slegrist, and C. Kloc, J.

**Cryst. Growth 290, 479**共2006兲.

15A. Moliton, *Optoelectronics* *of* *Molecules* *and* *Polymers*
共Springer, New York, 2005兲.

16A. A. Grinberg, S. Luryi, M. R. Pinto, and N. L. Schryer, IEEE
**Trans. Electron Devices 36, 1162**共1989兲.

17**J. A. Geurst, Phys. Status Solidi 15, 107**共1966兲.

18**R. Zuleeg and P. Knoll, Appl. Phys. Lett. 11, 183**共1967兲.

19*N. F. Mott and R. W. Gurney, Electronic Processes in Ionic Crys-*
*tals*共Clarendon, Oxford, 1940兲.

20S. Tavazzi, A. Borghesi, A. Papagni, P. Spearman, L. Silvestri, A.

Yassar, A. Camposeo, M. Polo, and D. Pisignano, Phys. Rev. B
**75, 245416**共2007兲.

21**S. Nešpurek and J. Sworakowski, J. Appl. Phys. 51, 2098**共1980兲.

22**O. Zmeškal, F. Schauer, and S. Nešpurek, J. Phys. C 18, 1873**
共1985兲.

23H. T. Henderson, K. L. Ashley, and M. K. L. Shen, Phys. Rev. B
**6, 4079**共1972兲.

24**R. H. Bube, J. Appl. Phys. 33, 1733**共1962兲.

25**J. Sworakowski and S. Nešpurek, IEEE Trans. Electr. Insul. 24,**
223共1989兲.

26**R. W. I. de Boer and A. F. Morpurgo, Phys. Rev. B 72, 073207**
共2005兲.